onto the tooth or packed inside a non-vital tooth. The
most effective material was considered hydrogen
peroxide . This bleaching agent made bleaching
treatments efﬁcient at removing intrinsic stains. Most
of the present-day vital bleaching materials contain
hydrogen peroxide in some form, or as carbamide
peroxide, which breaks down into hydrogen per-oxide
. Various methods of vital bleaching have been
developed and used over the years. In-ofﬁce bleaching
has been the most common technique during the last
20 years . In-ofﬁce bleaching is useful for removing
discolorations by using a high concentration of
hydrogen peroxide (35e38%). The dentist is in com-
plete control of the process throughout the treatment.
This provides the advantage of being able to terminate
the bleaching process at any time. Studies have shown
that higher concentration materials bleach teeth faster.
These materials usually work so rapidly that visible
results can be observed even after a single visit [8e10].
One important consideration with regard to a
restorative material is that the appearance of a restored
tooth can be spoiled by the restoration having a matt
surface ﬁnish, thus making it stand out from the rest of
the teeth. The simplest way to assess this is by visually
using an impression replica examined under a light
microscope or a scanning electron microscope (SEM).
It can also be numerically assessed by using a
Swift  and Haywood  reported that bleaching
techniques have no signiﬁcant effects on the color or
physical properties of porcelain or other ceramic ma-
terials, as well as amalgam or gold. Using a scanning
electron microscope [5,11], Bailey and Swift (4)
observed slight surface changes in microﬁlled and
hybrid composites after immersion for 4 h daily in
fresh bleaching gel . The SEM observations of
Turker and Biskin  showed only slight changes on
the surface of the restorative materials after home
bleaching. In a study by Wattanapayungkul et al. ,
the SEM images showed numerous cracks on the sur-
face of the restorative materials after home bleaching
The authors Turker and Biskin  and Wattana-
payungkul and Yap  also studied the effects of
bleaching on the surface roughness of restorative ma-
terials, and found no signiﬁcant difference in rough-
ness between the control and bleached groups.
To date, no literature data exists on bleaching with
25% hydrogen peroxide, or on the effects of bleaching
on currently-used dental restorative materials. There-
fore, this in vivo study evaluated the effects of in-ofﬁce
bleaching agents on the surface morphology of three
different aesthetic restorative materials.
2. Methods and materials
2.1. Patient selection
The research proposal and study design were
approved by the Aesthetical Committee of Research
and the IRB at Beirut Arab University. A total of 15
subjects, 18e45 year olds with one or more defective
class IV restoration or class IV caries, including the
labial surface of the maxillary anterior teeth, were
included in the study. Institutional Review Board (IRB)
consent forms were obtained from the patients.
The subjects were selected from the outpatient clinic
of the Faculty of Dentistry at the Beirut Arab University
according to the following exclusion criteria:
1. Subjects who had used bleaching products in the past
2. Subjects who were smokers.
3. Subjects who had had periodontal surgery or scaling
carried out in the previous six months.
4. Subjects with chronic periodontitis or signs of patho-
logical origin, or with radiographic signs of pulpal or
5. Subjects with severe medical complications that would
interfere with the study (liver disease, sensitivity to
peroxide products etc.).
6. Subjects with systemic diseases or who were taking
medication that caused tooth discoloration or Xerostomia.
7. Subjects with severe bruxism, tooth clenching, or un-
8. Subjects with tetracycline stains.
9. Subjects with a previously developed sensitivity to
hydrogen peroxide products (H2O2).
10. Any cavities where the gingival wall surpassed the
cement-enamel junction to ensure all the cavity walls
were on the enamel, or if a carious pulp exposure with
obvious bleeding occurred.
The preoperative clinical evaluation included com-
plete medical and dental histories, anterior maxillary
per apical radiographs, an assessment of pulp vitality
and tooth sensitivity, or any history of pain. The sub-
jects were informed about all the details of this
investigation and they signed IRB consent forms to
participate in this study.
All 15 subjects (36 restorations) were evaluated
before bleaching (baseline) after one week of restora-
tions prior to the bleaching treatment and then two
days, three months, six months, and one year after
bleaching. Evaluation was performed on the replica
169A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
impression for the restoration specimens in the patient's
mouth by using scan electron microscopy (SEM).
Out of the 15 subjects (36 restorations), only 12
subjects (30 restorations) remained; this number was
the basis for the statistical evaluations during the
follow-up periods. Three subjects were excluded for
not returning for examination two days after bleaching:
The ﬁrst subject had Beautiﬁl II, the second had
Ceram.x.mono, and the third had IPS Empress Direct
composite resin restorations. The number of restora-
tions evaluated at each recall is presented in Table 1.
The twelve subjects consisted of nine males and three
females between the ages of 28e30 years old.
The minimum specimen size required was ten
restorations in each group. Each group (n ¼ 4 sub-
jects) consisted of three subjects, who had three upper
anterior teeth defective class IV restorations, or class
IV caries, and one subject had one upper anterior
teeth lesion. They were restored with the same
restoration material type, and divided into three
groups according to the type of restoration material.
Three groups of resin composite materials were used
in this study: Beautiﬁl II1
, IPS Empress Direct2
2.3. Cavity preparation
The conservative cavity preparations were set to be
conservative in outline, just to include the defective
areas which were prepared using number 330 Carbide
Burs. The class IV preparations all had margins in the
dentin, they had butt-joint preparations, and all the
enamel margins were beveled. No base or liner was
used, except in deep cavities, where, based on our
judgment, an indirect pulp capping was considered
necessary. In these cases, the deepest part of the cavity
was covered with a thin layer of calcium hydroxide
. Shade A1 was selected for all the restorations to
counter any tooth color changes after bleaching; the
cavity was etched with 37% phosphoric acid4
applied and left undisturbed for 20 s, the air was
thinned for 5 s, and the light cured for 40 s using a
light curing unit5
with an intensity of 350 mW/cm2
Then the cavities were restored incrementally using
the three above mentioned restorative materials, and
were placed according to the manufacturer's in-
structions under complete rubber dam isolation.
Finishing and polishing of the restoration was car-
ried out during the same visit using medium, fine, and
superfine polishing discs6
with a slow-speed hand
piece rotating in one direction using the three-step
technique . The restored teeth were checked for
high points with articulating paper (Table 1). All the
subjects underwent oral prophylaxis within two weeks
before the placement of the restorations.
2.4. Surface texture measurement
To eliminate bias, The SEM evaluations were per-
formed by one blind examiner; they were evaluated
and classiﬁed into three categories: Without any
change (À), with minor/slight changes (þ), or with
major/severe changes (þþ). The criteria that differ-
entiated the minor from the major changes are as fol-
lows: Minor/slight changes were those that showed
negligible changes in surface texture. These changes
would not require any replacement of the restorations
in clinical practice.
Major/severe changes were those that showed a loss
of resin parts, or even surface cracks in addition to an
alteration in surface morphology. A washing out of the
composite surface meant a major change in surface
morphology. The major changes were those that were
detrimental to the material, and would require
replacement of that material if used in a restoration
Number of restorations evaluated at each recall examination.
Materials T0 T1 T2 T3 T4
Bea 12 10 10 10 10
IPS 12 10 10 10 10
Cer 12 10 10 10 10
Bea: Beautiﬁl II group, IPS: IPS Empress Direct group, Cer:
Ceram.x.mono group, T0: Before bleaching, T1: After two days of
bleaching, T2: After 3 months of bleaching, T3: After 6 months of
bleaching, T4: After one year of bleaching.
Bisphenylglycidyl Dimethacrylate (Bis-GMA), 7.5% Triethylen-
glycol Dimethacrylate (TEGDMA), 5% Aluminoﬂuoro, 70% Al2O3
(borosilicate glass), DL-Camphorquinone, (Shofu Dental Corporation,
Is a paste of Dimethacrylates, copolymer 20e21%wt, barium
glass 77.5e79%wt, (550 nm), initiators, stabilizers, and pigments,
(Ivoclar Vivodent, USA).
Is made up of methacrylate modiﬁed polysiloxane, dimethacry-
late resin, BaeAl-borosilicate glass 70%, pyrogenic SiO2 57%,
camphorquinone, ethyl-4-diemthylamino benzoate, a UV stabilizer,
and butylated hydroxy toluene, (DeTrey, Dentsply, Germany).
(Dentsply Detrey) for 15 s and then rinsed with water for 20 s and
blot dried. Prime and Bond NT (Dentsply Detrey).
(GNATUS, Fotopolimerizador optilight plus, Brazil).
(Sof-Lex system; 3M ESPE).
170 A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
The replica surface7
had no preliminary information
about the type of restorations. The surface morphology
of the restorative materials was evaluated by using the
replica at the following times: Before bleaching, then
two days, three months, six months, and one year after
bleaching. The measurements were recorded according
to the timetable as shown in Table 1.
The selection of a tooth specimen in each subject
was randomly assigned for either Beautiﬁl II, IPS
Empress Direct, or Ceram.x.mono composite restora-
tion (Table 1).
2.5. Replica Impresion technique
The replica impressions were taken from each pa-
tient; a primary impression was taken of the maxillary
arch using alginate8
, into which stone9
The resulting cast was used to construct a special
perforated tray without palatal coverage to ensure
consistent positioning of the replica impression into the
subject's mouth by using heavy body impression ma-
terials, and then then by reapplying this trial impres-
sion into the subject's mouth ﬁlled with light body
. If the catalyst and paste were
mixed too vigorously, air bubbles might have accu-
mulated in the replica. To correct this problem a very
thin layer was applied initially. This was followed by a
second layer over the original layer in order to
strengthen and ensure a ﬂatter base to the replica, into
was poured, thus ensuring that all
points in any given area were within working distance
of the analyzer. This technique provided an image of
the surface topography of each specimen.
2.6. Bleaching procedures
Bleaching was performed using (Zoom bleaching
gel) at 25% H2O2 and a Zoom Light Source12
cording to the manufacturer's instructions. After the
last cycle, all the bleach gel material was removed
from the subject's mouth using high-speed suction; the
teeth were rinsed with water for about 30 s . At the
end of every follow-up test procedure (before bleach-
ing, two days after bleaching, three months after
bleaching, six months after bleaching, and one year
after bleaching time); the specimens' replica were
attached to aluminum stub faces around the samples
for better light reﬂection during the SEM procedures
[21,22]. The specimens' replica were then sputter-
coated with carbon, and the representative areas were
examined, with the surface topography evaluation
recorded under a scanning electron microscope13
3.1. Surface texture analysis
Scanning electron microscope (SEM) examinations
of the restorative materials after bleaching showed
observable surface changes on the bleached surfaces
and after various application times. Regarding the
bleaching agents, their effect on surface texture of the
three restorative materials differed according to the
type and the time of the follow up.
Surface texture was classiﬁed as a percentage of
change in surface roughness using a three-category
scale where (À) was no change, (þ) was minor
changes, (þþ) was major changes. (P1) represents the
comparison between the three composite resin groups
(Bea, IPS, and Cer) at the same time period, while (P2)
represents the comparison between the same composite
resin group at different time periods in relation to the
baseline. A Chi-square test (c2
) was used to test the
qualitative data (Table 2) and SEM micrographs were
also presented (Figures 1 to 9).
Comparison between the three composite resin
There was a statistically highly signiﬁcant differ-
ence in the percentage of change in surface texture
among the three composite resin groups after bleaching
at all the time periods (P<0.01).
Comparison within the group at the different time
periods in relation to the baseline before bleaching
The Bea group revealed a statistically signiﬁcant
difference in the percentage of change in surface
texture after bleaching at all the tested time periods.
The IPS group did not show a statistically signiﬁcant
difference at all the time periods, except at one year
there was a statistically signiﬁcant change. The Cer
group did not show a statistically signiﬁcant difference
in the percentage of change in surface texture at all the
tested time periods (Table 2).
(Epoxy resin, Quick mast 105, Ayla Construction Chemicals,
(Major Prodotil Dentari, S.P.A, Italy).
(Elite Stone, Italy).
(3M ESPE, Express™ Registration Material, 6160J).
(Quickmast 105, Ayla Constraction Chmicals, DCP).
(Discus Dental, USA). 13
(Seron Technologies, AIS2100C).
171A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
Figures (1e9) show representative SEM micro-
graphs of the surface textures of the replicas of each
group before bleaching, two days after bleaching, and
at 1 year at same magniﬁcation (1000x). No major
changes were found for all the composite resin groups
at all the time periods after bleaching. However, some
minor changes were found for each group when
compared to the before bleaching micrographs.
Chi-square test results [P1 comparison between the three groups (Bea,
IPS and Cer) at the same time period, P2 comparison between the
same group at the different time period in relation to baseline].
Groups T0 T1
e þ þþ P2 e þ þþ P2
Bea 100% 0 0 P > 0.05 80% 20% 0 P ¼ 0.031*
IPS 100% 0 0 P > 0.05 90% 10% 0 P ¼ 0.305
Cer 100% 0 0 P > 0.05 100% 0 0 P > 0.05
P1 P > 0.05 P < 0.01**
Groups T2 T3
- þ þþ P2 - þ þþ P2
Bea 80% 20% 0 P ¼ 0.031* 70% 30% 0 P ¼ 0.017*
IPS 90% 10% 0 P ¼ 0.305 90% 10% 0 P ¼ 0.305
Cer 100% 0 0 P > 0.05 100% 0 0 P > 0.05
P1 P < 0.01** P < 0.01**
- þ þþ P2
Bea 70% 30% 0 P ¼ 0.017*
IPS 80% 20% 0 P ¼ 0.031*
Cer 90% 10% 0 P ¼ 0.305
P1 P < 0.01**
*Signiﬁcant difference at p < 0.05 level, **High signiﬁcant difference
at P < 0.01 level.
Bea: Beautiﬁl II group, IPS: IPS Empress Direct group, Cer:
score (À): Without any change, score (þ): With minor/slight change,
score (þþ): With major/severe change.
T0: Before bleaching, T1: Two-days after bleaching, T2: Three-months
after bleaching, T3: Six-months after bleaching, T4: One-year after
Fig. 1. SEM micrograph of Beautiﬁl II replica before bleaching
Fig. 2. SEM micrograph of Beautiﬁl II replica two-days after
bleaching (1000x magniﬁcation).
Fig. 3. SEM micrograph of Beautiﬁl II replica one-year after
bleaching (1000x magniﬁcation).
172 A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
These changes were in the form of increased
notches and surface porosity. Before bleaching, the
SEM micrographs of all the composite resins used in
this study revealed regular surface morphology with no
visible porosity or cracks (Figs. 1, 4 and 7). At two
days after bleaching, some porosities were seen in the
Beautiﬁl II and IPS Empress Direct replica micro-
graphs (Figs. 2, 5 and 8). No obvious changes were
found in the Ceram.x.mono replica micrographs. At
one year after bleaching, the three representative SEM
micrographs of the composite resin replicas revealed
some irregulars and porosities as indicated by the ar-
rows (Figs. 3, 6 and 9).
Fig. 10 represents a comparison between the three
composite resin types regarding the percentage of minor
changes in surface texture (þ) versus no change (À).
Minor changes were observed in 30% of the Bea group,
20% of the IPS group, and 10% of the Cer group.
Fig. 4. SEM micrograph of IPS Empress Direct replica before
bleaching (1000x magniﬁcation).
Fig. 5. SEM micrograph of IPS Empress Direct replica two-days
after bleaching (1000x magniﬁcation).
Fig. 6. SEM micrograph of IPS Empress Direct replica one-year
after bleaching (1000x magniﬁcation).
Fig. 7. SEM micrograph of Ceram.x.mono replica before bleaching
173A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
The purpose of this in vivo study was to evaluate the
effects of Zoom gel-bleaching agents on the surfaces of
three different aesthetic restorative materials, as well as
the effects of different follow-up times on the three
different surface treatment situations.
Light can be reﬂected from a surface, such as from a
mirror, or scattered in all directions. In this case the
surface is an ideal reﬂecting polished surface, while it
is not the case in a matt scattering surface. Whether a
material has a shiny or a matt surface texture is (more
importantly) a function of how smooth the surface is
Few studies have been performed that deal with the
effects of bleaching agents on restorative materials.
However, it is difﬁcult to compare the results of these
studies due to the variety of restorative materials used.
For this study, we know of no published studies that are
available on the effects of bleaching on some of the
restorative materials used in this study. In addition, in
the literature, only a few publications were found that
addressed the effects of in-ofﬁce bleaching on the
surface texture of restorative materials .
According to the SEM micrographs, Zoom gel 25%
H2O2 was found to have a mild effect on the surface
materials. The alterations observed on the surfaces of
the restorative materials were primarily found to be
slight changes and material-dependent.
The results of this study do not concur with those of
previous studies [4,12,23e25].
Schemehorn et al.  found no signiﬁcant effects
of 6% hydrogen peroxide on the surface morphology
of the hybrid composite being tested. A study by
Duschner et al.  revealed no signiﬁcant deleterious
effects on the restoration surfaces from 6% hydrogen
peroxide. Wattanapayungkul and Yap  only found
slight differences in surface roughness between the
control and bleached groups after in-ofﬁce bleaching
They also found differences between the materials,
varying somewhat, depending on the treatment proce-
dure. Wattanapayungkul et al.  showed that resin-
based restoratives may be signiﬁcantly roughened by
the extended use of bleaching agent. Their results,
however, were found to be material-dependent, which
Fig. 8. SEM micrograph of Ceram.x.mono replica two-days after
bleaching (1000x magniﬁcation).
Fig. 9. SEM micrograph Ceram.x.mono replica one-year after
bleaching (1000x magniﬁcation).
Fig. 10. In vivo surface texture percentage change for the three
174 A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
is in line with the results of this study. The Ceram.-
x.mono composites were not signiﬁcantly affected by
bleaching, while the Beautiﬁl II and IPS Empress
Direct composites showed changes in roughness, and
the SEM images revealed minor changes. Bailey and
Swift  demonstrated that at-home bleaching agents
(10% carbamide peroxide) caused only slight changes
(some areas with cracking) to the surface of the micro-
ﬁlled composite after immersion in fresh bleaching gel
for 4 h daily.
In a study by Turker and Biskin , the SEM
ﬁndings showed that the surface roughness of the
micro-ﬁlled composite was not affected by different
carbamide peroxide concentrations (10e16%). In the
same study, although there were no signiﬁcant differ-
ences in surface roughness (with respect to the con-
trols) for the micro-ﬁlled composite tested, the SEM
micrographs showed extensive shallow pitting local-
ized in the center, which was considered worse than
after treatment with Nite White and Rembrandt
bleaching agents when compared to treatment with
This diminution suggested that the bleaching agents
caused erosion on the surface of the composite matrix.
Bailey and Swift  suggested that the surface changes
could be caused by complex interactions within multi-
component bleaching products . The roughening
was suggested to result from the loss of the matrix,
rather than the ﬁller particles . Wattanapayungkul
et al.  suggested that the differences between the
materials could be a result of the difference in the resin
matrix components and the ﬁller size . Langsten
et al.  reported that a higher-concentration
carbamide peroxide bleaching agent, used as intended
by the manufacturer, posed no signiﬁcant risk to resin
composite restoration surfaces.
Most of the products used in previous studies were
home systems and over-the-counter bleaching prod-
ucts. The apparent discrepancies might be explained, in
part, by differences in experimental methodologies and
the bleaching agents used. While some researchers
adopted clinically relevant protocols, others employed
continuous exposure of the restorative materials to the
bleaching agents over stipulated periods [12,27,28].
The frequent change of bleaching agents may also
contribute to the disparity in the results.
In this study, the only material not inﬂuenced by the
bleaching agent was Ceram.x.mono. This bleaching
agent caused minor alterations to the surface of the
specimens' replicas to such a degree that the polished
restorations by this material should be not replaced
after bleaching, as the bleaching was carried out with
the Zoom light bleaching agent. The presence of pre-
reacted glass ionomer on the surfaces as inorganic
ﬁllers of the Beautiﬁl II composite might be the reason
that this material is more susceptible to alterations
during the bleaching procedure.
In addition to the Beautiﬁl II composite, the SEM
micrographs showed that the specimens' replicas from
the IPS Empress Direct composite became smoother
when they were treated with 25% hydrogen peroxide
for 45 min. Additionally, it was found that the speci-
mens' replicas from the Beautiﬁl II and the Empress
Direct composites, when treated with 25% hydrogen
peroxide, showed minor changes earlier than Ceram.-
x.mono. The results pertaining to the Beautiﬁl II
composite may be due to the different composition of
every composite. The total content of the inorganic
ﬁllers of the Beautiﬁl II composite is higher (83%wt)
than IPS Empress Direct (79%wt) and Ceram.x.mono
The differences in effects were more pronounced in
the cases of a higher concentrated solution (25%
hydrogen peroxide). Bleaching gels contain a variety
of aqueous solvents, any of which could contribute
alone or in combination with other components to
decrease the solubility of the resin matrix. Hydrogen
peroxide, in turn, breaks down into free radicals, which
eventually combine to form molecular oxygen and
water. Some aspect of this chemical process might
accelerate the hydrolytic degradation of resin com-
posites, as described by S€oderholm . Another
aspect may be that hydrogen peroxide and free radicals
have an effect on the resin ﬁller interface and cause a
ﬁller matrix debonding, thereby leading to changes in
the surface roughness . It is important to note that
the results are material-dependent, as some tooth-
colored materials are more susceptible to alterations,
and some bleaching agents are more likely to cause
these alterations .
The latter may be attributed to the differences in pH
between the bleaching agents . This study showed
that the composite composition and ﬁller type have an
important inﬂuence on the effects of bleaching on the
surfaces of the materials. The Ceram.x.mono compo-
sition and ﬁller type were found to be more stable than
the Beautiﬁl II and IPS Empress Direct composites.
Alterations to the surfaces of the Beautiﬁl II specimens'
replicas were found to be fewer when compared to the
alterations observed to the IPS Empress Direct speci-
mens' replicas. This could be explained by the fact that
the matrix-ﬁnished unpolished surfaces are polymer-
rich , and that this layer is relatively unstable
[33,34]. In contrast, the ﬁnished polished surfaces are
175A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
ﬁller glass-rich and more characteristic of the bulk
The effects of bleaching gels on the surface
roughness of nano-ﬁlled composite resins on bovine
enamel was evaluated by Wang et al.  using three
different bleaching agents: 35% hydrogen peroxide
Whiteness HP, 35% Whiteness HP MAXX, and 16%
carbamide peroxide Whiteness Standard. They found
that bleaching gels affected nano-ﬁlled and micro-
hybrid composite resins. The enamel was the surface
least affected. They concluded that surface roughness
alterations were material and time dependent.
It is vital to point out that within the limitations of
an in vivo experiment, the parameter of the monomer
leaching of the composite materials into the oral cavity,
the effect of saliva PH, tooth-brushing methods, and
the effects of oral cavity thermal changes all had an
effect on the restoration surfaces.
The surface of the Beautiﬁl II and IPS Empress
Direct specimens' replicas used in this study were
altered only slightly after bleaching with 25%
hydrogen peroxide. Bleaching did not change the sur-
face of the Ceram.x.mono specimens' replicas. This
agrees with the ﬁndings of Turker & Biskin . It is a
fact that Zoom bleaching gel is a very powerful
bleaching agent compared to different concentrations
of the others, which may explain the slight changes on
the surfaces of the Beautiﬁl II and IPS Empress Direct
specimens' replicas because of this bleaching agent.
Additionally, the way the Beautiﬁl II and IPS Empress
Direct specimens were polished might explain these
changes, even though we were polishing with Sof-Lex
discs for this kind of restoration.
1. The effects of in-ofﬁce bleaching on the surface
morphology of tooth-colored materials was mate-
rial and time dependent.
2. The composition, ﬁller type, size, and distribution
had an important inﬂuence on the effects of
bleaching on surfaces.
3. Beautiﬁl II and IPS Empress Direct were found to
be smoother compared to the Ceram.x.mono
specimens in terms of the detrimental effects of
4. In clinical situations, the restorative materials
required no replacement of the restorations after
bleaching with Zoom bleaching gel 25%, or
changes to their surface morphology, such as
staining, the formation of bioﬁlm, and bacterial
5. After bleaching with the Beautiﬁl II composite
resin the restorations after time may need surface
repolishing, while this is not needed after bleach-
ing with IPS Empress Direct and Ceram.x.mono
composite resin restorations.
6. Surface roughness is an effective tool to assess the
surface changes of materials and the behavior of
different types of compositons.
7. The result of surface roughness according to the
composition of the materials.
8. The changes in surface roughness are small and
considered clinically not signiﬁcant by the effects of
bleaching; however, they are signiﬁcant by aging.
9. Replicas are more related to qualitative rather than
quantitative measurements and they represent the
changes in the tooth-restoration surface.
10. Further and longer follow-up studies are recom-
mended at two or three years.
11. These results explain the absence of cracking
during surface roughness.
12. Measurements (AFM micrographs) and surface
13. Increasing smoothness representing a healthier
The in-ofﬁce Zoom gel agent does not cause
changes that would demand a replacement of the res-
torations when the agents have been applied onto the
surfaces of the aesthetic dental restorative materials.
 Paravina R, Johnston W, Powers J. New shade guide for evalu-
ation of tooth whitening colorimetric study. J Esthetic Restor
 Arens D. The role of bleaching in esthetics. Dent Clin N. Am J
 Lefever D, Ricardo J, Mercade M, Basilio J, Roig M. Optical
integration and ﬂuorescence a comparison among restorative
materials with spectrophotometric analysis. Quintessence Int J
 Bailey S, Swift Jr E. Effects of home bleaching products on
composite resins. Quintessence Int 1992;23(7):489e94.
 Haywood Van B. History, safety, and effectiveness of current
bleaching techniques and applications of the night guard vital
bleaching technique. Quintessence Int J 1992;23(7):471e88.
 FasanaroTom S. Bleaching teeth: history, chemicals, and
methods used for common tooth discolorations. J Esthetic Restor
 Al Shethri S, Matis B, Cochran M, Zekonis R, Stropes M. A
clinical evaluation of two in-ofﬁce bleaching products. Operative
Dent J 2003;28(5):488e95.
176 A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177
 Leonard R, Sharma A, Haywood V. Use of different concentra-
tions of carbamide peroxide for bleaching teeth: an in vitro study.
Quintessence Int J 1995;29(8):503e7.
 Auschill T, Hellwig E, Schmidale S, Hannig M, Rweiler N.
Effectiveness of various whitening techniques and their effects
on the enamel surface. Schweiz Monatsschr Zahnmed
 Auschill T, Hellwig E, Schmidale S, Hannig M, Arweiler N.
Efﬁcacy, side effects and patients' acceptance of different
bleaching techniques. Oper Dent 2005;30(2):156e63.
 Swift Jr E. Restorative considerations with vital tooth bleach-
ing. J Am Dent Assoc 1997;128:60Se4S.
 Turker S, Biskin T. Effect of three bleaching agents on the
surface properties of three different esthetic restorative mate-
rials. J Prosthet Dent 2003;89(5):466e73.
 Wattanapayungkul P, Yap AU, Chooi K, Lee M, Selamat R,
Zhou R. The effect of home bleaching agents on the surface
roughness of tooth-colored restoratives with time Operative
Dentistry Journal 2004;29(4):398e403.
 Wattanapayungkul P, Yap AU. Effects of in-ofﬁce bleaching
products on surface ﬁnish of tooth colored restorations. Oper-
ative Dent J 2003;28(1):15e9.
 Deliperi S, Bardwell D, PAPATHANASIOU A. Clinical eval-
uation of combined in-ofﬁce and take-home bleaching system. J
Am Dent Assoc 2004;135(5):628e34.
 Rosin M, Schwahn C, Kordass B, Konschake C, Greese U,
Teichmann D, et al. Multipractice clinical evaluation of an
Ormocer restoration 2 years results. Quintessence Int J
 Manuja N, Passi S, Pandit I, Singh N. Management of a case of
Ectodermal Dysplasia. J Dent Child 2011;78(2):107e10.
 Polydorou O, Hellwig E, Auschill T. The effect of different
bleaching agents on the surface texture of restorative materials.
Operative Dent J 2006;31(4):473e80.
 Swift E. Effects of bleaching on tooth structure and restorations,
part IV : effects on restorative materials. J Esthetic Restor Dent
 Jorgensen M, Carroll W. Incidence of tooth sensitivity after
home whitening treatment. J Am Dent Assoc
 Marder A. Replication microscopy techniques for NDE. ASM
 Lopes M, Costa L, Consani S, Gonini A, Sinhoreti M. Scan
electronic microscopic evaluation of marginal sealing on
composite restorations using different photo activation and
composite insertion methods. Indian J Dent Res
 Joiner A. The bleaching of teeth: a review of the literature. J
 Schemehorn B, Gonzalez-Cabezas C, Joiner A. A SEM evalu-
ation of a 6% hydrogen peroxide tooth whitening gel on dental
materials in vitro. J Dent 2004;32:35e9.
 Duschner H, Gotz H, White D, Kozak K, Zoladz J. Effects of
hydrogen peroxide bleaching strip gels on dental restorative
materials in vitro: surface microhardness and surface
morphology. J Clin Dent 2004;15(4):105e11.
 Langsten R, Dunn W, Hartup G, Murchison D. Higher con-
centration carbamide peroxide effects on surface roughness of
composites. J Esthetic Restor Dent 2002;14(2):92e6.
 Monaghan P, Lim E, Lautenschlager E. Effect of home
bleaching preparations on composite resin color. J Prosthet
 Cullen D, Nelson J, Sandrik J. Peroxide bleaches: effect on
tensile strength of composite resins. J Prosthet Dent
 S€oderholm K, Zigan M, Ragan M, Fischlschweiger W,
Bergman M. Hydrolytic degradation of dental composites. J
Dent Res 1984;63(10):1248e54.
 Swift Jr E, Perdigao J. Effects of bleaching on teeth and res-
torations. J Compend Continuing Educ Dent
 Price R, Sedarous M, Hiltz G. The pH of tooth-whitening
products. J Can Dent Assoc 2000;66(8):421e6.
 Kao E. Inﬂuence of food-simulating solvents on resin com-
posites and glass-ionomer restorative cement. Dent Mater J
 Hachiya Y, Iwaku M, Hosoda H, Fusayama T. Relation of ﬁnish
to discoloration of composite resins. J Prosthet Dent
 Shintani H, Satou J, Satou N, Hayashihara H, Inoue T. Effects
of various ﬁnishing methods on staining and accumulation of
streptococcus mutants HS-6 on composite resins. Dent Mater J
 Wang L, Francisconi L, Teresa M, Rodrigo J, Natali N,
Gonini A, et al. Effect of bleaching gels on surface roughness of
nanoﬁlled composite resins. Eur J Dent 2011;5(2):173e9.
177A.H. Al-Ameedee et al. / Tanta Dental Journal 12 (2015) 168e177